2CREVICE CORROSIONNarrow openings, gaps, spaces, pores etc. between metal-metal components or metal-non-metal components may provoke localized corrosion.NOTE: unintentional crevices (seams, cracks etc.) can also act in the same wayPassive alloys (especially stainless steels) are more vulnerable than more active alloys.
3Crevice corrosion at a metal-to-metal crevice site formed between components of type 304 stainless steel fastener in seawater
4Crevice Corrosion occurring on a Test specimen of Type 316 SS (Stainless Steel) in Acid Condensate Zone of a Model SO2 Scrubber.
5Crevice corrosion is caused by the existence of small volumes of stagnant (corrosive) solution. Small holes, gasket surfaces, lap joints, bolt or rivet heads, nuts, washers, surface deposits all can cause C.C. (Crevice Corrosion).Type 304 SS sheet can be cut by stretching a rubber band around it, immersing it in seawater (Fontana). The crevice between the rubber and the metal acts as the cutting zone.
6MECHANISMConsider riveted metal section, immersed in aerated seawater (pH 7) e.g. stainless steelAlthough O2 within crevice is rapidly used up, corrosion continues, controlled by overall cathodic reaction outside the crevice.Tendency to build up M+ within the crevice must be balanced by -ve charge diffusing in.Some OH- diffuses in, alot of Cl- diffuses in (OH- more mobile, c.f. FONTANA* … less of it).
7Reduction: O2 + 2 H2O + 4 e- 4 OH- MECHANISMOxidation: M M+ + e-Reduction: O H2O e- 4 OH-*FONTANA says Cl- more mobile … this is wrong.
9Most metal ions (except alkali metals) hydrolyze: M+ + H2O MOH + H+Both Cl- and H+ accelerate metal dissolution (Cl- breaks down oxide, also H+ partly responsible).NOTE: there is now the possibility for H2 evolution within the crevice maybe!NOTE: solution within crevices exposed to neutral dilute NaCl has been seen to have 3-10x [Cl-] in bulk, pH of 2-3.
11Factors that can affect Crevice Corrosion resistance of stainless steels GeometricalType of crevice:metal to metalnonmetal to metalCrevice gap (tightness)Crevice depthExterior to interior surface area ratioMetallurgicalAlloy composition:major elementsminor elementsimpuritiesPassive film characteristicsElectrochemical reactions:Metal dissolutionO2 reductionH2 evolution
13CREVICE CORROSION OF CU ALLOYS different from that of SS; attack occurs OUTSIDE the crevice “Crevice corrosion” of Alloy 400 (70 Ni - 30 Cu) after 45 Days in Natural Seawater
14Cathodic conditions inside crevices of Cu alloy have been inferred from observations of deposited Cu metal (where?).“Differential metal-ion concentration” has been invoked as the mechanism; greater concentration inside the crevice raises the potential and makes it more noble than the outside.Also, variant of the oxygen depletion mechanism has been invoked.Clearly the situation is complex.NOTE: ALL MATERIALS ARE SUSCEPTIBLE TO C.C. (CREVICE CORROSION), GIVEN NARROW CREVICES, POSSIBILITY OF CONCENTRATING IONS, DIFFERENTIAL AERATION CELLS, DIFFERENTIAL METAL CONCENTRATION CELLS, ETC.
15COMBATING CREVICE CORROSION (after Fontana) Methods and procedures for combating or minimizing crevice corrosion are as follows:Use welded butt joints instead of riveted or bolted joints in new equipment. Sound welds and complete penetration are necessary to avoid porosity and crevices on the inside (if welded only from one side).Close crevices in existing lap joints by continuous welding, caulking, or soldering.Design vessels for complete drainage; avoid sharp corners and stagnant areas. Complete draining facilitates washing and cleaning and tends to prevent solids from settling on the bottom of the vessel.
16COMBATING CREVICE CORROSION (after Fontana) Inspect equipment and remove deposits frequently.Remove solids in suspension early in the process, if possible.Remove wet packing materials during long shutdowns.Provide uniform environments, if possible, as in the case of backfilling a pipeline trench.Use "solid," nonabsorbent gaskets, such as Teflon, wherever possible.Weld instead of rolling in tubes in tube sheets.
17FlLIFORM CORROSIONAlthough not immediately apparent, filiform corrosion (filamentary corrosion occurring on metal surfaces) is a special type of crevice corrosion.In most instances it occurs under protective films, and for this reason it is often referred to as underfilm corrosion.This type of corrosion is quite common; the most frequent example is the attack of enameled or lacquered surfaces of food and beverage cans that have been exposed to the atmosphere. The red-brown corrosion filaments are readily visible.
18Filiform corrosion usually on metals covered with thin organic film (0.1 mm) BUT also reported for: steel;magnesium;aluminum;tin;silver;gold;phosphate;enamel;as well as with organics (lacquer, paper; seen on paper-backed Al foil, between metal and paper).
19A lacquered steel can lid exhibiting filiform corrosion showing both large and small filaments partially oriented in the rolling direction of the steel sheet. Without this 10 x magnification by a light microscope, the filiforms look like fine striations or minute tentacles; (often mistaken for biologically – induced corrosion).
20Attack usually occurs when relative humidity between 65 and 90%; has been seen at lower R.H. (Relative Humidity).Average filament width mm .. depending on coating (thickness, porosity, etc.), R.H., and corrosiveness of environment (presence of SO2, H2S, etc.).Filament height 20 m. Growth rates observed between 0.01 mm/d and 0.85 mm/d.Filaments are like minute tunnels, full of corrosion products.
21Liquid in “head” is typically acidic. . . . pH 1- 4. IN ALL CASES.... O2 (or air) and water are needed to sustain filiform corrosion … indicates a form of a DIFFERENTIAL AERATION CELL.Discuss:differential aeration cellconcentration cell.
22An aside on differential aeration . . (differential) concentration cell remember example: remember Cu - alloy crevice:Attack usually begins at imperfections in coating e.g., cuts, knicks, pores, etc.CO2 can stimulate process by dissolving in water carbonic acid.Chlorides, SO42-, S2- which can dissolve in condensing atmospheric moisture also increase attack.Optimum temperature for filiform attack between 20 & 35C.(potential log [Cu+])
23Effect of humidity on filiform corrosion of enameled steel Relative humidity, % AppearanceNo corrosionVery thin filamentsWide corrosion filamentsVery wide filamentsMostly blisters, scattered filiformBlistersSource: M. Van Loo, D. D. Laiderman, and R. R. Bruhn, Corrosion, 9:2 (1953).Appearance:Schematic diagram of a corrosionfilament growing on aniron surface (magnified).
24Schematic diagrams illustrating the interaction between corrosion filaments: (a) Reflection of a corrosion filament;(b) splitting of a corrosion filament;(c) joining of corrosion filaments;(d) “death trap”.
25MechanismHead supplied with H2O by osmosis (high concentration of Fe2+ inside) through coating and from precipitated hydroxide/oxide. Oxygen reduction creates hydroxide; precipitation creates corrosion product tail further oxidation to Fe3+ oxide etc. Hydrolysis of salts in head creates acidic conditions.Details of mechanismnot understood………….e.g., why do filaments“reflect” off other filaments? etc.
26Filiform Corrosion on PVC-Coated Al Foil Advancing head and cracked tail of a filiform cell.Scale: mmGelatinous corrosion products oozing out of porous tail section.Scale: m
27Close-up of the advancing head shown in adjacent figure Close-up of the advancing head shown in adjacent figure. Minute cracks can be seen at the head/tail interface of a filiform corrosion cell. These cracks are entry points for water and air to provide a source of hydroxyl ions and an electrolyte. Intermediate corrosion products are just beginning to form in the head, and they undergo further reaction to form an expanded tail. The tail region is a progressive reaction zone that ultimately forms spent corrosion products. Between the head and porous end, ions gradually react with water and oxygen and are slowly transported in the direction of the tail to form final corrosion products.Scale: m
28Prevention NOT EASY....store coated metals in dry air;use more brittle films these should crack at head and destroy differential aeration;use impermeable coatings.
30Pitting CorrosionPITTING: Extreme localized attack, may perforate metal sheet/plate etc.“Pitting factor” =d = average penetration from weight loss;p = deepest penetration“Undercutting”pit opening usually < 1 mm.Pits may overlap to give the appearance of rough, general wastage.
31“incubation” period may be months or years. Pitting is an insidious and destructive form of corrosion:difficult to detect (pits may be small on surface, but extensive below surface from undercutting; may be covered with deposit);can cause equipment to fail (by perforation) with very little weight loss;difficult to measure as pit depth and distribution vary widely under (nominally) identical conditions;“incubation” period may be months or years.
32Pitting of 18-8 stainless steel by acid-chloride solution. Pitting of stainless steel condenser tube.
33Pits usually occur on upward-facing horizontal surfaces, and less frequently on vertical surfaces;rarely on downward-facing surfaces;pit growthpit growthGravity is involved.pit growth
34Mechanism: Has some features in common with CREVICE CORROSION.... consider metal M being pitted by aerated NaCl solution...Autocatalytic processes occurring in a corrosion pit.
35Remember:inside pit - anodic, rapid dissolution;outside pit - cathodic, O2 reduction;most M+ will hydrolyse, form H+;positive charges attract Cl- ions;H+ and Cl- accelerate metal dissolution;high ionic concentrations in pit make O2 solubility very low;high density of solution within pits means pits are more stable when growing downwards;static environment accelerates process.
36At high pH (i.e., high OH- concentration), precipitation of iron hydroxides and oxidation to Fe3+ oxides can lead to corrosion product caps or tubes around pits on steels.Corrosion tube growth mechanism.
37ETCHED or GROUND surfaces more likely to pit than polished surfaces. Metals Susceptible to PittingMost often, passivating metals, especially stainless steels, often in passivating environments (e.g., containing oxygen) but with agents such as Cl- that attack the passive oxide film.SENSITIZED SS particularly vulnerable (its heat treatment has depleted the grain boundaries of Cr by precipitating chromium carbide).COLD WORKING increases pitting attack, perhaps dislocation pattern is important.DISCUSSETCHED or GROUND surfaces more likely to pit than polished surfaces.Stainless Steel more susceptible than Carbon Steel (though CS will have more rapid GENERAL CORROSION).
38Element Effect on pitting resistance Some alloys developed especially to resist pitting.Effects of alloying on pitting resistance of stainless steel alloysElement Effect on pitting resistanceChromium IncreasesNickel IncreasesMolybdenum IncreasesSilicon Decreases; increases when present with molybdenumTitanium and niobium Decreases resistance in FeCI3, other mediums no effectSulfur and selenium DecreasesCarbon Decreases, especially in sensitized conditionNitrogen IncreasesSource: N. D. Greene and M. G. Fontana, Corrosion 15:25t (1959).
39Pitting EnvironmentsUsually, solutions containing chloride or chlorine-containing ions (e.g., hypochlorites [bleaches]) have strong pitting tendencies.Bromides are also aggressive, but fluorides and iodides are not.Cupric, ferric and mercuric ions promote pitting easily reduced cathodically and do not require dissolved O2; CuCl2 and FeCl3 are extremely aggressive (latter used as a test solution).Thiosulphate ion (S2O32-) may also promote pitting.
40Evaluating Pitting Attack Weight loss of test specimens no good ( why ?).Measurement of pit depth complicated because of statistical variations.Average pit depth of little use, since it is the deepest pit that causes failure.Relationship between pit depth and the number of pits appearing on a corroded surface.
41MAXIMUM PIT DEPTH can be a useful way of expressing pitting corrosion, and for comparing pitting resistance of standard test samples.HOWEVER, statistical nature of pitting means that sample size is important.Should never predict lifetime of plant components from tests on small samples.Pit depth as a function ofexposed area.
42Examples of pitting corrosion: Alloy-800 SG tubes with phosphate chemistry…pitting severe pitting wastage.Point Lepreau had some pitting, switched to AVT.SS cooling water H.X. left static under silted conditions…severe pitting; replaced with Ti plate-type.Others?